Tissue Engineering of
28.1 The Native Heart Valve as a Design Goal. . . . . . . . . . . . . . . 28-2
Anatomy and Terminology • Microstructure and Material
Behavior • Valvular Cells
28.2 Approaches to the Tissue Engineered Heart Valve . . . . 28-6
Biodegradable Polymeric Scaffolds • Decellularized Leaﬂet
Scaffolds • Cell Seeding • Natural Materials • Building
Block Approach • Cell Origin • Bioreactors for
Conditioning and Proof of Concept • In Vivo Testing in
Animal Models • Clinical Experience
28.3 Conclusions and Future Challenges . . . . . . . . . . . . . . . . . . . . 28-13
K. Jane Grande-Allen Deﬁning Terms . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 28-14
Rice University References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 28-15
Heart valves are essential to the normal function of the heart and cardiovascular/cardiopulmonary systems.
When functioning properly, the heart valves allow unrestricted, unidirectional blood ﬂow through the
heart for subsequent distribution throughout the body. Consequently, valve disease or dysfunction can
result in signiﬁcant harm, as the reduction in the forward ﬂow of blood limits the oxygenation of the tissues
and can induce cardiac, cardiovascular, or cardiopulmonary compensation. Valve disease is prevalent in
our society, with valve replacement or repair in approximately 90,000 people in the United States in 2001
 (275,000 worldwide ). Moreover, valve disease can be either congenital or acquired. For example,
approximately 9 to 14 of every 10,000 children born are affected with the Tetralogy of Fallot [3,4],
a congenital heart disorder characterized by a narrowing of the pulmonary valve among other anomalies.
Acquired valve disease can affect people of all ages and may be due to an infectious agent (rheumatic
heart disease, endocarditis), systemic diseases (lupus, carcinoid syndrome), other cardiac disease, trauma,
pharmacologic agents, aging-related changes, or many other causes, some of which remain unknown .
The majority of current treatments for heart valve disease involve elective surgical replacement of
the valve with a mechanical, bioprosthetic, or cryopreserved allograft (homograft) valve. The allograft
is the treatment of choice for children, because bioprosthetic valves will calcify rapidly in children and
mechanical valves cannot grow with the child . Aortic and pulmonary allografts have also been used very
successfully in adults, with the pulmonary conduit having a 90% freedom from replacement at 20 years
, but the vascular remnant of these allografts eventually calciﬁes. Unfortunately, allografts, much like
other donated organs, are in scarce supply. Moreover, allografts needs to be matched to the recipient tissue
type to prevent immunological rejection , which narrows the diminishing pool of donated organs
28-2 Tissue Engineering
even further. Alternative options such as mechanical or bioprosthetic heart valves can be used in many
situations, and are widely available, but have their own limitations . Mechanical heart valves require
anticoagulation therapy, which some patients cannot tolerate. Bioprosthetic valves do not require any
anticoagulation, but do not contain any living tissues, and they undergo stiffening, calciﬁcation, and
structural deterioration in vivo as a result of their glutaraldehyde ﬁxation during manufacturing .
Bioprosthetic valves demonstrate a freedom from structural deterioration of 49% at 10 years and only
32% at 15 years,  and eventually require another surgical replacement. Overall, there is great need
for a living, unﬁxed tissue-engineered heart valve (TEHV) or valved conduit in adults who require valve
replacements. A TEHV with the potential for growth would also provide pediatric patients with a superior
alternative for the treatment of valve defects.
28.1 The Native Heart Valve as a Design Goal
28.1.1 Anatomy and Terminology
The aortic valve is one of four valves in the heart, but it is replaced most frequently, and therefore will be
discussed in greater detail. The aortic valve consists of three pieces of connective tissue (the right, left, and
noncoronary leaﬂets) that are attached to the aorta at one edge, and are free to move at the other edge.
These free edges meet centrally to close the valve and keep the blood from reentering the left ventricle. The
valve is located in the bulbous base of the aorta, which is known as the aortic root (an anatomic recreation
for a TEHV is shown in Figure 28.1). There are several distinct anatomic regions of the valve leaﬂet itself
(Figure 28.2). The leaﬂet attachment edge inserts into the aortic root wall at the crown-shaped annulus
. The common region where two leaﬂets insert into the root wall is their commissure. The leaﬂet
belly, or body, is the main portion of the leaﬂet (0.4 mm thick in humans ), and bears the majority
of the pressure load when the valve is closed . The coaptation area is the 0.5 to 0.6 mm thick 
region of the leaﬂet that is in contact with the two other leaﬂets when the valve is closed. The free margin
is the unattached edge of the leaﬂet, and suspends the leaﬂet between the tops of the commissures, much
like cables of a suspension bridge [10,13]. Finally, the central portion of the edge of the valve leaﬂet is the
Nodule of Arantius, a thickened area (0.95 to 1.2 mm ) that helps maintain valve closure .
The pulmonary valve (the other “semilunar” valve) is located in the pulmonary root between the right
ventricle and pulmonary artery, and is thinner and more delicate than but otherwise almost identical to the
aortic valve. The semilunar valves are quite different structurally from the “atrioventricular” valves. The
mitral valve consists of two differently shaped leaﬂets attached at their outer border to the junction between
the left atrium and left ventricle. The free edges and ventricular surfaces of the leaﬂets are connected to
the papillary muscles of the left ventricle by numerous chordae tendineae. Likewise, the tricuspid valve is
located between the right atrium and right ventricle. The tricuspid valve also contains chordae, but has
three differently shaped leaﬂets as opposed to two. The tricuspid leaﬂets and chordae are thinner, shorter,
and more delicate than those in the mitral valve.
28.1.2 Microstructure and Material Behavior
The semilunar valve leaﬂets consist of three histologically deﬁned layers: the ventricularis forms the lower
surface, the ﬁbrosa forms the upper surface, and the spongiosa layer lies in between  (Figure 28.3 and
Figure 28.4). The ventricularis contains a meshwork of elastic ﬁbers along with loosely scattered collagen
ﬁbers . The predominant elastic makeup allows this layer to expand in response to tension in the
closed state of the valve, and then retract when the valve opens in response to ventricular ejection .
The ﬁbrosa contains collagen ﬁbers (predominantly type I), which are aligned largely circumferentially,
although radially aligned ﬁbers are found near the root-valve annulus . The collagen ﬁber bundles
in the ﬁbrosa serve as the main source of strength for the diastolic pressure. The ridged appearance
of the ﬁbrosa is attributed to a corrugation of that tissue layer, in addition to the collagen bundles
. The spongiosa is a gelatinous layer containing loose connective tissue that is rich in proteoglycans
Tissue Engineering of Heart Valves 28-3
FIGURE 28.1 PGA/P4HB scaffold after cell seeding and 2 weeks of bioreactor conditioning. (Reprinted from
Hoerstrup, S.P., Sodian, R., Daebritz, S., Wang, J., Bacha, E.A., Martin, D.P., Moran, A.M., Guleserian, K.J.,
Sperling, J. S., Kaushal, S., Vacanti, J.P., Schoen, F.J., Mayer, J.E., Circulation, 102, III-46, Copyright 2000, with
permission from Lippincott Williams & Wilkins.)
(PGs), and serves as a mechanism for compressive resistance  and shear between the ﬁbrosa and
The mitral and tricuspid valves have a similar laminated structure, except the respective outer layers are
“upside down” from the arrangement shown in Figure 28.3. In these valves, the thick, heavily collagenous
layer is located on the ventricular side, whereas the thin, predominantly elastic layer is found on the atrial
side; these layers are also separated by a spongiosa. These similarities, which may be beneﬁcial in future
tissue engineering of atrioventricular valves, end with the chordae tendineae, which are not found in
semilunar valves. The chordae are strong, thin, cable-like structures that contain a core of highly aligned
collagen inside a thin outer sheath of elastic ﬁbers and endothelial cells.
The interaction between the extracellular matrix (ECM) constituents within the valve microstructure
allows distensibility, strength, elastic recovery, viscoelasticity, and an even distribution of deformation over
a wide range of loading . Like many other biological soft tissues, the stress–strain and load elongation
curves of heart valve tissues are characterized by a low pretransition elastic modulus at initial strain (due to
elastic ﬁbers), followed by a transition zone to a higher posttransition elastic modulus at higher strains (due
to the uncrimped collagen) . The unique collagen and elastic ﬁber arrangements in the different layers,
however, bestow the leaﬂet with anisotropic behavior (Figure 28.5). The greater circumferential stiffness
(due to collagen) contributes to normal aortic valve function by restricting downward leaﬂet motion,
while the lower radial stiffness permits the inward motion toward leaﬂet coaptation. This properly closing
aortic valve will allow blood ﬂow from the left ventricle into the ascending aorta, and prevent reverse
ﬂow. During this functional cycle, the leaﬂets interact with complex patterns of blood ﬂow , and are
28-4 Tissue Engineering
(a) Commissures (2 of 3)
Nodule of arantius
(b) Free margin
FIGURE 28.2 Semilunar valve leaﬂet anatomy. (a) Illustration of aortic valve leaﬂets within an opened aortic root.
(b) Single valve leaﬂet.
FIGURE 28.3 The histological layers of the aortic valve leaﬂet. Movat’s Pentachrome stain. F, ﬁbrosa; S, spongiosa;
subjected to transvalvular pressures as high as 120 mmHg  and shear stresses as high as 7.9 Pa .
These magnitudes of load are lower in the pulmonary circulation, where the transvalvular pressure across
the pulmonary valve is only 25 mmHg .
28.1.3 Valvular Cells
Heart valves contain both endothelial and interstitial cells [21–23]. The valvular endothelial cells (VECs)
populate the outer surfaces of the valves, whereas “interstitial cells” are all the cells that populate the inside
Tissue Engineering of Heart Valves 28-5
FIGURE 28.4 Illustration of the histological layers of the valve during systole and diastole. (Reprinted from
Schoen, F. J., J. Heart Valve Dis., 6, 2, Copyright 1997, with permission from ICR Publishers.)
Fibrosa Ventricularis Fibrosa Vertricularis
fresh fresh fresh fresh
cirumferential cirumferential radial radial
0 20 40 60 80 100
FIGURE 28.5 Radial and circumferential stress–strain curves of the ventricularis and ﬁbrosa of aortic valve leaﬂets.
(Reprinted from Vesely, I. and Noseworthy, R., Micromechanics of the ﬁbrosa and the ventricularis in aortic valve
leaﬂets, J. Biomech., 25, 107, Copyright 1992, with permission from Elsevier.)
of the leaﬂets. Although it is presumed that the VECs provide the tissue with a nonthrombogenic sur-
face, their functions otherwise are only beginning to be explored [23,24]. The valvular interstitial cells
(VICs), which are only slightly better understood, are responsible for the synthesis of extracellular matrix
components, including collagen, elastin, proteoglycans, and hyaluronan (for reviews see References 25
and 26). A key characteristic of VICs is that this group of cells exhibits a mixed phenotype of both ﬁbro-
blastic and smooth muscle cell characteristics and are yet uniquely different from both these cell types
[21,22,27,28]. It remains unclear whether this dual phenotype is caused by a single population of cells
that express both features simultaneously [22,27], a single population of cells that can switch between
these two phenotypes , or a population of several types of cells [29,30]. The different phenotypes of
VICs are typically distinguished by their morphological appearance and immunohistochemical staining
[21,27,28]. The ﬁbroblastic phenotype is marked by elongated cells that contain numerous organelles for
28-6 Tissue Engineering
matrix synthesis, and stain for prolyl-4-hydroxlyase. The smooth muscle cell phenotype is denoted by
cobblestone cells that stain for smooth muscle α-actin and stress ﬁbers. VICs display this dual phenotype
consistently throughout passaging [22,27]. Although in native valves these different cell phenotypes are
slightly segregated [29,30], cells harvested from different regions of the valve had a consistent dual phen-
otypic appearance and growth characteristics . It has also been difﬁcult to separate these phenotypes
in culture .
28.2 Approaches to the Tissue Engineered Heart Valve
The basic approach to constructing a TEHV, as with many other engineered tissues, is ﬁrst to seed an
appropriate cell type onto or within a suitable scaffold, and then to have a period of incubation during
which the cells remodel or otherwise become integrated with the scaffold, and form a neotissue. This deﬁn-
ition is intentionally ambiguous because a wide range of cells, scaffolds, and incubation environments
have been used. All of the proposed TEHVs, however, have been designed to have as many of the ideal
features of a heart valve substitute as possible [31,32] (i) maintain normal structural and biological func-
tion over the patient’s lifetime, (ii) not elicit any inﬂammatory, foreign body, or immunologic responses,
(iii) have antithrombotic surfaces and the potential for growth and self-repair, (iv) manufactured for each
individual, (v) easy to implant with little technical variability, and (vi) available in an unlimited supply
[31,32]. The majority of research of TEHVs has focused upon the structural, antithrombotic, immuno-
logic, and availability aspects of this lofty goal. Although the studies described here do not represent an
exhaustive discussion of TEHVs, several reviews provide more thorough detail [2,26,33].
28.2.1 Biodegradable Polymeric Scaffolds
Almost half of the proposed designs for TEHVs involve seeding cells on or within a polymeric biode-
gradable scaffold. The purpose in using a biodegradable scaffold is to anchor the seeded cells within an
environment that is originally strong enough to withstand the in vivo mechanical forces, yet will sub-
sequently degrade slowly, thereby transferring the function of load-bearing to the nascent ECM produced
by the cells. Ideally, scaffold degradation rate and cellular synthesis rate should be balanced so that the
scaffold has been completely degraded when the seeded cells have generated an amount of ECM compar-
able to native heart valves. The scaffold should also have initial material properties that are comparable to
The ﬁrst such scaffold used to generate a TEHV was a woven mesh of 90% poly(glycolic acid)
(PGA)/10% poly(lactic acid) (PLA) sandwiched between nonwoven PGA mesh, which was seeded with
ovine vascular myoﬁbroblasts and endothelial cells and used to replace the right leaﬂet of the pulmonary
valve in a lamb model . Although the resulting pulmonary valve was functional in the short term
(3 weeks), this scaffold was found to be too stiff and thick for long-term use [35,36]. Conversely, seeding
cells in PGA mesh alone produced a neotissue that was too delicate to handle , although the high
porosity of this scaffold (95%) encouraged high seeding efﬁciencies and subsequent ECM production .
To avoid the mechanical limitations of the previous scaffolds, Sodian et al.  developed a new TEHV
scaffold using poly(hydroxyalkanoate) (PHA), a thermoplastic, easily moldable polymer. The polymer was
cast into a valved-conduit-shaped mold, made porous through a salt leaching process, and seeded with
autologous ovine vascular myoﬁbroblasts and endothelial cells. Although this valved conduit functioned
normally in a sheep model for up to 17 weeks, the PHA scaffold material did not degrade fully by that time,
and the developing neotissue did not contain any histologically detectable elastin or have an endothelial
cell coating . Moreover, PHA has a high echocardiographic density, which prevented the TEHV
performance from being evaluated by Doppler echocardiography.
Because the PHA did not degrade rapidly enough, valved conduits were next assembled from nonwoven
PGA mesh coated with a thin layer of poly-4-hydroxybutyrate (P4HB), a biodegradable thermoplastic
moldable polymer that provided the nonwoven PGA with additional strength . After seeding with
Tissue Engineering of Heart Valves 28-7
(a) (b) (c)
FIGURE 28.6 After 6 weeks in vivo (a), the TEHV from Figure 28.5 demonstrates preliminary organization (50×).
After 16 weeks (b) and 20 weeks (c), the TEHV leaﬂet demonstrates organized, dense collagen on the outﬂow
surface, elastic ﬁbers on the inﬂow surface (arrow), and spongy organization within (both 100×). (Reprinted from
Hoerstrup, S. P., Sodian, R., Daebritz, S., Wang, J., Bacha, E.A., Martin, D.P., Moran, A.M., Guleserian, K.J.,
Sperling, J. S., Kaushal, S., Vacanti, J.P., Schoen, F.J., Mayer, J.E., Circulation, 102, III-48, Copyright 2000, with
permission from Lippincott Williams & Wilkins.)
autologous ovine vascular cells and 2 weeks of dynamic conditioning in a bioreactor (Figure 28.1), these
TEHVs were implanted in the pulmonary position of sheep for 20 weeks. These TEHVs functioned well,
with only mild to moderate pulmonary regurgitation at 16 and 20 weeks. Upon explant, the TEHV leaﬂets
were found to have the normal three-layered structure of native heart valves (Figure 28.6), although their
biochemically measured concentrations of collagen, elastin, and GAGs, as well as their ultimate tensile
strength, were signiﬁcantly higher than normal native pulmonary leaﬂets. Overall, the PGA/P4HB has
been considered a very successful scaffold for TEHV development and is still being investigated [40,41].
Other biodegradable scaffolds that have been explored include biodegradable polyurethane, which was
found to have not degraded completely at 6 weeks . Finally, new classes of biodegradable scaffolds
are being designed, such as a combination of poly(vinyl alcohol) (PVA) with brush groups of modiﬁed
PLA . This novel scaffold should combine the advantages of PVA, a high water content hydrogel with
high elasticity and the ability to incorporate biologically active molecules on its hydroxyl groups, with the
features of PLA, which is biodegradable, can be crosslinked, and is hydrophobically attractive to cells.
28.2.2 Decellularized Leaﬂet Scaffolds
Although polymeric biodegradable scaffolds have a long history in TEHV designs, another early approach
that is still in active development today is the use of decellularized semilunar valve leaﬂets as a scaffold, with
the rationale that they would provide the requisite strength , and already contain ECM in the correct
microstructural arrangement . Unlike polymeric designs, there is no need to fabricate or mold these
scaffolds. Moreover, removing the cells would presumably eliminate the most antigenic elements, thereby
avoiding any immunological response in the recipient. This reasoning has enabled the development
of decellularized scaffolds from not only human heart valves (from donated allograft organs [45–47] or
cadavers ), but also porcine heart valves. The predominant matrix element in these scaffolds, collagen,
is highly conserved between species and is thus considered minimally antigenic [49,50], although there
are concerns about the potential for transmission of xenogenic diseases .
A major area of research in the development of this scaffold is determining the best method to remove
the cells from the original valve leaﬂet. Several different methods, involving ionic and nonionic detergents,
28-8 Tissue Engineering
solutions that are hypotonic or hypertonic, and enzyme treatments, have been attempted, abandoned,
debated, and revisited, with only few direct comparisons . In early studies, a treatment involving
hypotonic saline to lyse the cells followed by two washes with the nonionic detergent Triton X-100 and
one enzymatic soak in DNAse and RNAse was effective in the removal of all cells and cell debris [44,53].
This method preserved the majority of the thermal, physical, and material properties with the exception
of a slight swelling and a slight increase in the stress relaxation of the tissue. This successful treatment was
in contrast to their previous experimentation with the ionic detergent sodium dodecyl sulfate (SDS), in
which the leaﬂet matrix swelled up to three times and had signiﬁcant thermal denaturation . On a
single wash basis, however, SDS appears to remove more cells than Triton X-100 . A combination of
0.5% trypsin and 0.2% EDTA was also successful in removing cells from human and porcine valves [48,55],
as was a solution of 1% deoxycholic acid . A solution of 0.1% N -cetylpyridinium chloride was shown
to remove cells effectively and to preserve the tissue’s microstructure and mechanics but this treatment
induced calciﬁcation when the decellularized leaﬂet was tested in a rat subcutaneous dermal model .
Booth et al.  found that solutions of 0.03 to 0.1% SDS and 0.5% Na deoxycholate in hypotonic solutions
worked best (with SDS causing a slight increase in tissue extensibility ), which they attribute to better
protease inhibition than in the previous studies that implicated SDS in ﬁber damage. Although a few
studies reported using protease inhibitors [48,53,55], such as phenylmethyl sulfonyl ﬂuoride (PMSF) and
EDTA, to block the endogenous lysosomal proteases released during cell lysis and to prevent degradation
of the matrix scaffold, certain protease inhibitors (including PMSF) are short-lived in aqueous solutions
and a more stable compound such as aprotinin may be preferable . Many studies did not report any
use of protease inhibitors, which could result in partial degradation of the collagen and elastic matrix
components of the scaffold. The partial degradation of elastin in these scaffolds is considered particularly
risky given that decellularized aortic wall, found to contain an abundance of partially degraded elastin,
was prone to calciﬁcation in a rat subcutaneous dermal model .
Once prepared, the decellularized leaﬂet scaffold is almost always reseeded with autologous cells derived
from the same host animal to be used in the TEHV study. Several of these scaffolds have been reseeded
with endothelial cells only [56,60]. The main intent of this seeding is to form an antithrombotic coating
around the bare collagen , and is an especially important consideration in planning for human TEHV
use, because humans may have a more difﬁcult time endothelizing structures than do the sheep models
used in most of these studies . Many other decellularized scaffolds, however, have also received a
preliminary reseeding with vascular myoﬁbroblasts in attempts to accelerate the eventual remodeling of
the matrix [51,55,62–64]. Despite the preliminary seeding of the decellularized scaffolds, dispersing the
cells within the existing matrix has proven difﬁcult, with some tendency for the cells to remain on the
surface or to merely line the largest pores . In addition, Steinhoff et al.  found that the seeded cells
tended to make new matrix on top of as opposed to within the existing scaffold matrix.
The Synergraft™ valve (Cryolife, Inc., Kennesaw, Georgia) consists of a decellularized porcine pul-
monary root or composite aortic root (constructed from three noncoronary root-valve segments);
decellularized human allografts are also available [46,66]. In contrast to the other approaches, the Syner-
graft valved conduits were not reseeded with any cells before implantation in sheep models, but became
entirely repopulated with host cells and were completely functional for one year . Although these scaf-
folds were developed with many techniques similar to those used for other TEHVs, they are not universally
considered tissue-engineered structures because they are not reseeded with cells before implantation.
28.2.3 Cell Seeding
The methods used to seed the cells on and within the polymeric biodegradable scaffolds and the decellu-
larized valve leaﬂets tend to be very straightforward: a concentrated solution containing the cells is dripped
onto the scaffold surface and the cells disperse by gravity [67,68]. This seeding dispersion was encouraged
by gentle agitation in some studies , but there was no report of any improved seeding efﬁciency due
to this method. Many TEHVs have been developed by seeding ﬁrst with myoﬁbroblasts (several million
cells), incubating 10 to 14 days, and then seeding with endothelial cells [34,37,38,62,69–72]. In preparation
Tissue Engineering of Heart Valves 28-9
for this staged seeding process, a mixed population of vascular cells can separated into endothelial and
nonendothelial cells using ﬂuorescence-activated cell sorting (FACS)-based binding to acetylated low-
density lipoprotein (positive binding in endothelial cells ). Staged seeding is not necessarily required
; mixed vascular cells seeded onto PGA/PLA–PGA sandwich scaffolds tended to segregate during
incubation and in vivo implantation, forming neotissue with endothelial cells (staining for Factor XIII) on
the outside and myoﬁbroblasts (negative for Factor XIII) within. Other factors shown to improve seeding
efﬁciency include 24 or 36 h seeding intervals (as opposed to 2 or 12 h intervals ), using polymeric
scaffolds with high porosity such in PGA [67,68], mixing soluble collagen into the cell seeding solution
, and coating the scaffold with Matrigel before seeding .
28.2.4 Natural Materials
Although the majority of TEHVs to date have been constructed from either biodegradable polymeric or
decellularized leaﬂet scaffolds, there are a number of alternative scaffolds that have been developed using
natural polymers such as collagen. The rationale behind using these natural materials is that the synthetic
biodegradable polymers may have cytotoxic degradation products such as lactic acid, which can lower
the pH of the culture medium . A very early approach, reported by Carpentier et al. , was to
inject solubilized collagen into a leaﬂet shaped mold. The resulting valve was implanted in sheep in the
tricuspid or mitral position and functioned for up to 10 months without incompetence. Upon explant,
ﬁbroblasts were found within the collagen leaﬂets, but the leaﬂets were determined to have thickened
slightly in vivo. More recently, valvular interstitial cells seeded within collagen sponge scaffolds were
found to demonstrate phenotypic characteristics very similar to cells within intact valve leaﬂets .
Rothenburger et al. [71,75] grew human and porcine vascular and valvular cells within a freeze-dried
porous type I collagen matrix in vitro and found that the cells produced the large hydrating proteoglycan
(PG) versican, the small collagen-binding PG decorin, ﬁbronectin, thrombospondin, and a medium-
sized heparan sulfate PG (possibly perlecan or syndecan). The production of these PGs and glycoproteins
indicate that the cells were interacting with and organizing the nascent ECM. Another natural material,
ﬁbrin, is being explored as a natural scaffold because ﬁbrin gels can be made autologously from a patient’s
own blood and thereby prevent an immunologic reaction [67,68,76]. Fibrin gel components can also be
coupled with exogenous biologically functional groups, such as growth factors, for improved neotissue
formation. In addition, the use of injection molding to cast a cell-seeded ﬁbrin gel ensures that the cells
will be evenly distributed throughout the TEHV. This initial even distribution of cells is an advantage
over the seeding of ﬁbrous or sponge structures, where seeding dispersion is due to gravity and barely
50% of cells attach . The disadvantage with ﬁbrin gels is their initial weakness, which needs to be
improved before in vivo studies can be performed. Yet another natural polymer that has been proposed
is chitosan, a polysaccharide derivative that has been used for other tissue engineering applications .
Although three-dimensional chitosan scaffolds have yet to be tested in a TEHV, monolayer cultures of
VECs adhered better to chitosan surfaces — and chitosan/collagen IV combinations in particular — than
to PHA surfaces.
28.2.5 Building Block Approach
Almost without exception, the approach to TEHV development has been to use scaffolds that are destined
for degradation or remodeling by the cells that will populate these constructs. The exception to this
paradigm is the approach by Vesely et al. , in which the different ECM structural components are
derived and then assembled into an approximation of the native aortic valve microstructure in vitro. The
collagen bundles that provide the leaﬂet strength are replicated by neonatal rat aortic smooth muscle cells
(NRASMCs) seeded within a type I collagen gel and anchored to promote uniaxial or branched contrac-
tion. The lubricating glycosaminoglycan component will be represented by cross-linked hyaluronan (also
seeded with NRASMCs), and the network and sheets of elastic ﬁbers are synthesized by the NRASMCs atop
the crosslinked hyaluronan and around the collagen bundles. The ﬁnal valve structure will be assembled
28-10 Tissue Engineering
by stacking alternating layers of hyaluronan/elastic sheets with layers of collagen bundles/elastic sheaths
that are oriented as they would be in the native aortic valve (predominantly circumferential). This novel
approach is still in the in vitro developmental stages, but it is envisaged that the multiple layers would
compact, and the embedded cells would synthesize additional ECM, during a period of in vitro dynamic
28.2.6 Cell Origin
It is generally agreed that the source of cells for a TEHV should be autologously derived from the intended
valve recipient. This is particularly feasible given that most valve surgeries are elective, with criteria for
the decisions of surgical timing being continuously reevaluated [5,80]. Autologous cells may perform
best in pediatric cases, given that adult cells may have diminished proliferative ability (cell sources are
discussed extensively in Reference 2). The anatomic source of these autologous cells, however, has not
been ﬁrmly established. Shinoka et al.  determined that arterial myoﬁbroblasts were superior to
dermal ﬁbroblasts in generating a strong, collagen-rich, and organized neotissue; Schnell et al.  found
that venous cells were better yet. Given that saphenous veins are more easily harvested than arteries, the
use of venous cells was therefore considered a promising alternative to arterial cells for seeding a TEHV
scaffold. Although many studies continue to explore the use of cells derived from vascular sources, there
were two recent reports that used either the stromal cells  or mesenchymal stem cells  from bone
marrow. In the ﬁrst case, human bone marrow stromal cells (obtained from the sternum) were seeded on
a PGA/P4HB valved conduit, then conditioned in a bioreactor. After 14 days, the cells showed phenotypic
characteristics of myoﬁbroblasts (smooth muscle α-actin and vimentin), but did not show markers for
muscle, osteogenic, or endothelial differentiation. In the second case, ovine bone marrow mesenchymal
stem cells were seeded on the same type of valved conduit, then conditioned in bioreactor. Although
the differentiation characteristics such as cell phenotype were not reported, the cells were able to form a
functional neotissue in vitro.
Very few research groups have actually attempted to use VECs and VICs in the design of TEHVs
[30,75,78]. It appears to have been assumed, if not often explicitly postulated, that whatever cell type is
seeded within the TEHV will soon differentiate and begin to express the phenotypic characteristics of
valvular cells. With rare exception , this assumption has not been tested in any depth, even though
recent gene expression work has shown that VECs have many transcriptional differences from vascu-
lar endothelial cells . VECs were also four times more proliferative in culture than were vascular
endothelial cells , which may explain why vascular endothelial cells have frequently failed to form a
continuous endothelial coating of the TEHV scaffolds in vitro  or in vivo [38,44,63]. VICs seeded in
decellularized porcine leaﬂets differentiated and segregated into regionally speciﬁc myoﬁbroblasts, ﬁbro-
blasts, endothelial cells, and smooth muscle cells after 15 days in vitro . After seeding in porous collagen
sponge-like structures, VICs demonstrated phenotypic similarity to cells in native valve leaﬂets  and
produced many of the PGs normally found in valves  A potential source for autologous valvular cells
was proposed by Maish et al. , who found that valvular cells could be harvested from an ovine tricuspid
valve without compromising the function of the tricuspid valve in the donor animal. This option may be
important if the restoration of the VIC and VEC phenotype proves necessary and cannot be accomplished
using an alternative cell source.
28.2.7 Bioreactors for Conditioning and Proof of Concept
Bioreactors have been widely used to provide the developing TEHV with strength-building mechanical
stimulation prior to implantation within the animal model. Compared with static controls, bioreactor-
conditioned TEHVs have demonstrated greater production of collagen, greater cell densities, improved
mechanical strength, and more compact matrix organization [39,40,55]. It has also been proposed that
bioreactor conditioning maintains the synthesis of ECM and DNA at levels normally found in the valve
leaﬂets . Bioreactors can also accelerate the turnover of the biodegradable matrix. Incubation in
Tissue Engineering of Heart Valves 28-11
FIGURE 28.7 This bioreactor design creates pulsatile ﬂow by cyclically pumping air beneath the silicone diaphragm
separating the medium and air chambers. This action draws medium from a reservoir and propels it through the TEHV
ﬁxed to the silicone tubing above. (Reprinted from Hoerstrup, S.P., Sodian R., Sperling, J.S., Vacanti, J.P., Mayer J. E.,
Tissue Eng., 6, 1, Copyright 2000, with permission from Mary Ann Liebert, Inc.)
a dynamic ﬂexure bioreactor also augmented the bulk degradation of PGA/P4HB and PGA/PLA/P4HB
scaffolds, resulting in signiﬁcantly less ﬂexural stiffness at 3 weeks compared to unﬂexed controls .
The types of bioreactors developed for TEHV studies can be generally classiﬁed into one of two categories.
The ﬁrst category, which has a continuously circulating supply of tissue culture medium, is predomin-
antly used for the conditioning of intact TEHV and valved conduits. These bioreactors generally consist
of a medium reservoir, a chamber to hold the TEHV, a pressure source, ports for gas exchange, optional
pressure and ﬂow transducers, and often have components to mimic vascular compliance and resist-
ance [85,86] (Figure 28.7 and Figure 28.8). A similar setup was used in a study of the synthesis of
collagen, GAGs, and DNA by valvular cells . Because these bioreactor systems are capable of pro-
ducing pulsatile ﬂows ranging from 50 to 2000 ml/min  or even 20 l/min , and transvalvular
pressures of 10 to 240 mmHg, they can easily be tailored to the conditioning or testing of aortic or
pulmonary TEHVs. Feedback-driven tensioning systems have also been incorporated into these biore-
actors . The second category of bioreactor tends to be smaller and scalable, and is used more for
proof of concept studies that examine how mechanical stimulation can improve the TEHV charac-
teristics. An example of this was developed by Engelmayr et al. , in which scaffolds identical to
those used in certain TEHVs were subjected to ﬂexural conditioning, but were not bathed in circulating
28-12 Tissue Engineering
V TE valve
M Mechanical valve
LV LV Left ventricle
E External circuit
P Pressure transducer
FIGURE 28.8 A bioreactor ﬂow loop that includes components for variable compliance, resistance, and pressure
measurements. (Reprinted from Dumont, K., Yperman, J., Verbeken, E., Segers, P., Mauris, B., Vandenberghe, S.,
Flameng, W., Verdonck, P.R., Artif. Organs, 26, 711, Copyright 2002, with permission from Blackwell Publishing.)
28.2.8 In Vivo Testing in Animal Models
Although many potential TEHV designs have been successfully compared using in vitro and bioreactor
analyses, evaluation of the inﬂammatory, immunologic, and calciﬁc responses requires an in vivo model.
Canines have been used at least twice [44,88], but the majority of TEHVs have been tested in vivo in
the widely accepted ovine models (either lamb or mature sheep) . TEHVs have been implanted
into the atrioventricular position in the past , and a heterotopic implantation in the abdominal
aorta was recently reported , but most are tested in the pulmonary position, either as an orthotopic
replacement of the pulmonary valve [38,39,45,51,56,72] or heterotopically interposed between the main
and left pulmonary artery . Single [34,69] and double  leaﬂet replacements within the pulmon-
ary valve have been attempted with more success in the single leaﬂet replacement. The double leaﬂet
replacement involved two identical PGA/PLA–PGA sandwich scaffolds: one seeded TEHV leaﬂet and one
unseeded control. Unfortunately, this otherwise ingenious approach did not work because the stiff, thick
scaffolds were unable to coapt normally and cause pulmonary insufﬁciency . More recent TEHV
designs are often tested using a valved conduit, containing all three leaﬂets, in the orthotopic pulmonary
These in vivo studies have often demonstrated an early but very mild inﬂammatory response to the
TEHV , although this response was stronger when allogeneic as opposed to autologous cells were
seeded . A late inﬂammatory response (9 to 12 weeks) was reported with a reseeded decellularized
porcine TEHV . The remnant muscular shelf of decellularized leaﬂets has also been shown to invoke
a mild inﬂammatory and calciﬁc response . Otherwise, reports of calciﬁcation of the scaffolds have
been with mixed; there was heavy calciﬁcation of reseeded decellularized scaffolds after 12 and 24 weeks
in vivo , while a Synergraft decellularized porcine scaffold (not reseeded) showed no calciﬁcation after
21 weeks .
28.2.9 Clinical Experience
The majority of TEHVs have only been tested in vitro or in animal models; no TEHV has been approved
for clinical use in the United States. The porcine and human Synergrafts, which are technically not TEHVs
since they are not reseeded with cells, have been approved in the United States . As of 2003, these
decellularized human valved conduits have been implanted in more than 150 patients in the United States
and more than 1000 patients worldwide, approximately 84% of which have been in the pulmonary
position (16% aortic). The distribution of patient age in the United States has been approximately 1/3
children and 2/3 adults, with a mean follow-up time of 231 days (range 0 to 788 days). In the two cases
where these pulmonary allograft conduits were explanted (due to external ﬁbrosis at 14 months and
unrelated infection at 3 months), the leaﬂets and conduit had been repopulated with ﬁbroblasts and
Tissue Engineering of Heart Valves 28-13
myoﬁbroblasts and demonstrated an endothelial lining and normal leaﬂet architecture. Function of the
pulmonary Synergraft allografts have been comparable to cryopreserved allografts [46,61], whereas the
aortic Synergraft allografts have evoked humoral antibodies in 25% of patients, but have shown normal
aortic valve function with only trivial regurgitation . The porcine pulmonary Synergrafts have been
implanted in 20 patients , with 3 deaths and conduit pseudoaneurysm formation in 3 patients, but
14 other patients have had satisfactory valve performance for a maximum of one year. Unfortunately, the
porcine Synergraft has not been as successful in the pediatric population, with a massive inﬂammatory
response leading to leaﬂet degeneration and rupture in at least seven children in Austria and Norway .
One Synergraft that was examined after being implanted for one year showed no host recellularization
of the implant at all and the formation of a ﬁbrous capsule around the porcine tissue, which was very
different from the results in a sheep model , in which the entire leaﬂet was repopulated with cells after
In Germany, decellularized human cryopreserved pulmonary allografts that were reseeded with auto-
logous venous endothelial cells were implanted in at least 6 Ross procedure patients with a mean age of
44 years . All patients demonstrated an improvement of ejection fraction at 3 months. One patient
was reported to be excellent condition after 12 months, and had not demonstrated any fever during this
time. This absence of fever was interpreted as an absence of any antigenic inﬂammatory or immunologic
28.3 Conclusions and Future Challenges
There are many challenges ahead for the future of TEHVs. The ﬁrst challenge appears to be the recapitula-
tion of the many aspects of valvular biology in a living TEHV, particularly in designs involving nonvalvular
cells. Quite frankly, it remains to be determined if such recapitulation would even be necessary for TEHV
function, even though that ﬁnding could help direct future TEHV research. Moreover, the nascent ﬁeld
of valvular biology lags far behind vascular biology. Regardless, future TEHV research may wish to build
upon the many studies over the last several years that have examined the contractile, synthetic, signaling,
interactive, and diffusion characteristics of heart valves at the tissue, cellular, and molecular level. Normal
aortic valve leaﬂets and VICs, for example, will contract slowly in response to stimulation with vasoactive
agents such as serotonin, epinephrine, and endothelin-1 [28,89], potentially to maintain a baseline resting
tension in the normal aortic valve . More recently, the proliferative, migratory, synthetic, signal-
ing, and phenotypic transdifferentiation responses of VICs to members of the renin–angiotensin system
(including TGF-β) and vasoactive agents have been assessed [90–92]. Furthermore, the receptors and/or
mRNA for serotonin, angiotensin II, bradykinin, and angiotensin-converting enzyme have been identiﬁed
in VICs [92,93]. In fact, many of the transcriptional and proliferative characteristics of valvular cells have
been shown to be different from those expressed by vascular cells [24,93]. Cell–matrix interactions have
been demonstrated at the molecular level by the characterization of several integrins in bovine and baboon
VICs . Finally, oxygen diffusion within young porcine aortic valves was recently measured  and
it was observed that blood vessels were present in most regions of the valve thicker than 0.5 mm. This
ﬁnding highlights the differences between pediatric heart valves, which are vascularized [96,97] and even
innervated , and adult heart valves, which have far less nerves and vessels, but contain viable, synthetic
cells nonetheless. Exactly how well oxygen and nutrients diffuse to these adult VICs, and likewise to the
cells within a TEHV, is a fertile topic for further research.
Another challenge for the future is the development of TEHV replacements for the aortic, atrioventricu-
lar, and venous valves. The highest clinical need is for the aortic position. To meet the higher pressure
and ﬂow requirements of the systemic circulation, the current pulmonary TEHV designs will need to
be adapted to produce a stronger neotissue. In a recent proof of concept study that explored this need,
a PGA/P4HB scaffold seeded with human venous myoﬁbroblasts became more than three times stiffer
when the maximum cyclic strain was raised from 7 to 10% during bioreactor conditioning . Given
that the atrioventricular valves are more commonly repaired than replaced , recent TEHV work in
28-14 Tissue Engineering
that regard has focused on replacement components, as opposed to the entire valve. The chordae, in
particular, frequently rupture in prolapsed mitral valves ; torn chordae are currently replaced with
Gore-Tex™ sutures. Because these sutures are several times stiffer than normal chordae , Vesely
et al.  have been developing tissue-engineered chordae (large collagen ﬁber bundles) by seeding
NRASMCs in a type 1 collagen gel and allowing the cell-seeded gel to contract uniaxially. Although these
tissue-engineered chordae have not yet been tested in vivo, and are an order of magnitude less stiff than
normal native human chordae, they have approximately normal extensibility . As this avenue of TEHV
research is very young, these preliminary results are likely to improve substantially in the years to come.
Tissue engineered venous valves have been developed in a sheep model using allogeneic decellularized
jugular veins seeded with autologous venous myoﬁbroblasts and endothelial cells; these valves were still
patent at 12 weeks .
The ﬁnal challenge, particularly given the clinical reports of failure of the Synergraft valves in pediatric
patients , are the ethical considerations involved as these research ﬁndings are eventually translated to
clinical practice . Although there are no current governmental regulatory divisions that are focusing
exclusively on engineered tissues, U.S. and European regulatory agencies are planning centers that will
meet this need. Beyond that goal lies the problem of developing standards to which engineered tissues such
as the TEHV would be held. Furthermore, we are reminded by Sutherland and Mayer in their excellent
review of this topic, “compliance with standards alone carries no guarantee that a given device will be
free from risk” . Applying a risk management approach, with identiﬁcation and severity grading
of potential hazards, is an appropriate ﬁrst step along this path. Hazards particularly associated with the
current characteristics of the TEHV described in this chapter could be scaffold-related, such as adverse
reactions to the degradation products of the biodegradable scaffolds, or the potential for transmission
of porcine endogenous retrovirus from the decellularized porcine valve scaffold to the TEHV recipient
[51,102]. Other hazards could be related to the cells involved, particularly if they are not autologous, or
to the performance of the TEHV in vivo.
The ﬁeld of TEHV research is growing exponentially and has demonstrated many recent advances,
particularly in the development and application of bioreactor technologies. New research in valvular
biology and targeted scaffold development, together with frequent reﬂection and review [2,26,33], are
certain to drive this ﬁeld ahead. Although there are many hurdles to overcome before the many promises
of TEHVs become fully realized, the potential to create a living, healing, growing valve continues to inspire
signiﬁcant effort in this exciting ﬁeld.
Allogeneic: Taken from a different individual of the same species
Atrioventricular: Referring to the position between the atrium and the ventricle. The mitral and
tricuspid valves are atrioventricular valves.
Autologous: Taken or derived from the same individual.
Coaptation: Referring to contact between different heart valve leaﬂets, or regions of the leaﬂets where
this contact occurs when the valve is closed.
Ejection fraction: The percentage of blood pumped out of an individual’s left ventricle.
Heterotopic: Referring to a region of the body where a structure is not normally located.
Incompetence and insufﬁciency: Inability of the heart valve to close property.
Orthotopic: Referring to a region of the body where a structure is normallt located.
Ross Procedure: Surgical replacement of a patient’s deﬁcient aortic valve with a pulmonary autograft,
followed by implantation of a cryopreserved pulmonary allograft in the pulmonary position.
Semilunar: Referring to the half-moon shape of the leaﬂets of the pulmonary and aortic valves.
Tetralogy of Fallot: A congenital heart defect with four predominant symptoms (ventricular septal
defect, pulmonary valve stenosis, right ventricular hypertrophy, and malposition of the aorta over
Tissue Engineering of Heart Valves 28-15
Valvular interstitial cells: An all-encompassing term for the nonendothelial cells that are contained
within the heart valve leaﬂets. This deﬁnition includes cells of variable phenotype.
Xenogenic: Taken from a different species.
 American Heart Association, Heart Disease and Stroke Statistics — 2004 Update, American Heart
Association, Dallas, 2004.
 Rabkin, E. and Schoen, F.J., Cardiovascular tissue engineering, Cardiovasc. Pathol. 11, 305, 2002.
 American Heart Association, Youth and Cardiovascular Diseases — Statistical Fact Sheet, American
Heart Association, Dallas, 2004.
 Topol, E.J., Cleveland Clinic Heart Book, Hyperion, New York, 2000.
 Otto, C.M., Valvuar Heart Disease, 2nd ed., Saunders, Philadephia, 2004.
 Mayer, J.E. Jr., In search of the ideal valve replacement device, J. Thorac. Cardiovasc. Surg. 122, 8,
 Ross, D.N., Options for right ventricular outﬂow tract reconstruction, J. Cardiovasc. Surg. 13, 186,
 Vesely, I., Barber, J.E., and Ratliff, N.B., Tissue damage and calciﬁcation may be independent
mechanisms of bioprosthetic heart valve failure, J. Heart Valve Dis. 10, 471, 2001.
 Fann, J.I. et al., Twenty-year clinical experience with porcine bioprostheses, Ann. Thorac. Surg. 62,
 Mercer, L., Benedicty, M., and Bahnson, H., The geometry and construction of the aortic leaﬂet,
J. Thorac. Cardiovasc. Surg. 65, 511, 1973.
 Sahasakul, Y. et al., Age-related changes in aortic and mitral valve thickness: implications for
two-dimensional echocardiography based on an autopsy study of 200 normal human hearts, Am.
J. Cardiol. 62, 424, 1988.
 Christie, G.W. and Stephenson, R.A., Modelling the mechanical role of the ﬁbrosa and the ventricu-
laris in the porcine bioprosthesis, in Surgery for Heart Valve Disease, Bodnar, E., Ed., Heart Valve
Diseases, London, 1989, p. 815.
 Sutton, J.P. 3rd, Ho, S.Y., and Anderson, R.H., The forgotten interleaﬂet triangles: a review of the
surgical anatomy of the aortic valve, Ann. Thorac. Surg. 59, 419, 1995.
 Clark, R.E. and Finke, E.H., Scanning and light microscopy of human aortic leaﬂets in stressed
and relaxed states, J. Thorac. Cardiovasc. Surg. 67, 792, 1974.
 Sauren, A.A. et al., Aortic valve histology and its relation with mechanics — preliminary report,
J. Biomech. 13, 97, 1980.
 Vesely, I. and Noseworthy, R., Micromechanics of the ﬁbrosa and the ventricularis in aortic valve
leaﬂets, J. Biomech. 25, 101, 1992.
 Grande-Allen, K.J. et al., Glycosaminoglycans and proteoglycans in normal mitral valve leaﬂets
and chordae: association with regions of tensile and compressive loading, Glycobiology 14, 621,
 Sauren, A.A. et al., The mechanical properties of porcine aortic valve tissues, J. Biomech. 16, 327,
 Patton, H.D. et al., Textbook of Physiology. Circulation, Respiration, Body Fluids, Metabolism, and
Endocrinology, W.B. Saunders, Philadelphia, 1989.
 Weston, M.W., LaBorde, D.V., and Yoganathan, A.P., Estimation of the shear stress on the surface
of an aortic valve leaﬂet, Ann. Biomed. Eng. 27, 572, 1999.
 Taylor, P., Allen, S., and Yacoub, M., Phenotypic and functional characterization of interstitial cells
from human heart valves, pericardium and skin, J. Heart Valve Dis. 9, 150, 2000.
 Johnson, C.M., Hanson, M.N., and Helgeson, S.C., Porcine cardiac valvular subendothelial cells
in culture: cell isolation and growth characteristics, J. Mol. Cell. Cardiol. 19, 1185, 1987.
28-16 Tissue Engineering
 Cuy, J.L. et al., Adhesive protein interactions with chitosan: consequences for valve endothelial cell
growth on tissue-engineering materials, J. Biomed. Mater. Res. 67A, 538, 2003.
 Farivar, R.S. et al., Transcriptional proﬁling and growth kinetics of endothelium reveals differences
between cells derived from porcine aorta versus aortic valve, Eur. J. Cardiothorac. Surg. 24, 527,
 Taylor, P.M. et al., The cardiac valve interstitial cell, Int. J. Biochem. Cell. Biol. 35, 113, 2003.
 Flanagan, T.C. and Pandit, A., Living artiﬁcial heart valve alternatives: a review, Eur. Cell. Mater.
6, 28, 2003.
 Lester, W.M. and Gotlieb, A.I., In vitro repair of the wounded porcine mitral valve, Circ. Res. 62,
 Messier, R.H. et al., Dual structural and functional phenotypes of the porcine aortic valve
interstitial population: characteristics of the leaﬂet myoﬁbroblast, J. Surg. Res. 57, 1, 1994.
 Della Rocca, F. et al., Cell comparison of the human pulmonary valve: a comparison study with
the aortic valve — the VESALIO project, Ann. Thorac. Surg. 70, 1594, 2000.
 Bertipaglia, B. et al., Cell characterization of porcine aortic valve and decellularized leaﬂets repop-
ulated with aortic valve interstitial cells: the VESALIO project (Vitalitate Exornatum Succedaneum
Aorticum Labore Ingenioso Obtenibitur), Ann. Thorac. Surg. 75, 1274, 2003.
 Cohn, L.H. and Lipson, W., Selection and complications of cardiac valvular prostheses, in Glenn’s
Thoracic and Cardiovascular Surgery, Baue, A.E. et al., Eds., Appleton & Lange, Stamford, CT,
1996, p. 2043.
 Harken, D.E. and Curtis, L.E., Heart surgery — legend and a long look, Am. J. Cardiol. 19, 393,
 Stock, U.A. et al., Tissue engineering of heart valves — current aspects, Thorac. Cardiovasc. Surg.
50, 184, 2002.
 Shinoka, T. et al., Tissue engineering heart valves: valve leaﬂet replacement study in a lamb model,
Ann. Thorac. Surg. 60, S513, 1995.
 Sodian, R. et al., Evaluation of biodegradable, three-dimensional matrices for tissue engineering
of heart valves, ASAIO J. 46, 107, 2000.
 Kim, W.G. et al., Tissue-engineered heart valve leaﬂets: an animal study, Int. J. Artif. Organs 24,
 Zund, G. et al., The in vitro construction of a tissue engineered bioprosthetic heart valve, Eur. J.
Cardiothorac. Surg. 11, 493, 1997.
 Sodian, R. et al., Early in vivo experience with tissue-engineered trileaﬂet heart valves, Circulation
102, III22, 2000.
 Hoerstrup, S.P. et al., Functional living trileaﬂet heart valves grown in vitro, Circulation 102, III44,
 Hoerstrup, S.P. et al., Tissue engineering of functional trileaﬂet heart valves from human marrow
stromal cells, Circulation 106, I143, 2002.
 Engelmayr, G.C. Jr. et al., A novel bioreactor for the dynamic ﬂexural stimulation of tissue
engineered heart valve biomaterials, Biomaterials 24, 2523, 2003.
 Schnell, A.M. et al., Optimal cell source for cardiovascular tissue engineering: venous vs. aortic
human myoﬁbroblasts, Thorac. Cardiovasc. Surg. 49, 221, 2001.
 Nuttelman, C.R., Henry, S.M., and Anseth, K.S., Synthesis and characterization of photocross-
linkable, degradable poly(vinyl alcohol)-based tissue engineering scaffolds, Biomaterials 23, 3617,
 Wilson, G.J. et al., Acellular matrix: a biomaterials approach for coronary artery bypass and heart
valve replacement, Ann. Thorac. Surg. 60, S353, 1995.
 Goldstein, S. et al., Transpecies heart valve transplant: advanced studies of a bioengineered xeno-
autograft, Ann. Thorac. Surg. 70, 1962, 2000.
 Elkins, R.C., Is tissue-engineered heart valve replacement clinically applicable? Curr. Cardiol. Rep.
5, 125, 2003.
Tissue Engineering of Heart Valves 28-17
 Elkins, R.C. et al., Decellularized human valve allografts, Ann. Thorac. Surg. 71, S428,
 Cebotari, S. et al., Construction of autologous human heart valves based on an acellular allograft
matrix, Circulation 106, I63, 2002.
 Yannas, I.V., Natural materials, in Biomaterials Science. An Introduction to Materials in Medicine,
Ratner, B.D. et al., Eds., Academic Press, San Diego, 1996, p. 84.
 Miller, E.J., Chemistry of the collagens and their distribution, in Extracellular Matrix Biochemistry,
Piez, K.A. and Reddi, A.H., Eds., Elsevier, New York, 1984, p. 41.
 Leyh, R.G. et al., Acellularized porcine heart valve scaffolds for heart valve tissue engineering and
the risk of cross-species transmission of porcine endogenous retrovirus, J. Thorac. Cardiovasc.
Surg. 126, 1000, 2003.
 Booth, C. et al., Tissue engineering of cardiac valve prostheses I: development and histological
characterization of an acellular porcine scaffold, J. Heart Valve Dis. 11, 457, 2002.
 Courtman, D.W. et al., Development of a pericardial acellular matrix biomaterial: biochemical
and mechanical effects of cell extraction, J. Biomed. Mater. Res. 28, 655, 1994.
 Kim, W.G., Park, J.K., and Lee, W.Y., Tissue-engineered heart valve leaﬂets: an effective method of
obtaining acellularized valve xenografts, Int. J. Artif. Organs 25, 791, 2002.
 Schenke-Layland, K. et al., Complete dynamic repopulation of decellularized heart valves by
application of deﬁned physical signals — an in vitro study, Cardiovasc. Res. 60, 497, 2003.
 Dohmen, P.M. et al., Ross operation with a tissue-engineered heart valve, Ann. Thorac. Surg. 74,
 Spina, M. et al., Isolation of intact aortic valve scaffolds for heart-valve bioprostheses: extracellular
matrix structure, prevention from calciﬁcation, and cell repopulation features, J. Biomed. Mater.
Res. 67A, 1338, 2003.
 Korossis, S.A., Fisher, J., and Ingham, E., Cardiac valve replacement: a bioengineering approach,
Biomed. Mater. Eng. 10, 83, 2000.
 Bailey, M.T. et al., Role of elastin in pathologic calciﬁcation of xenograft heart valves, J. Biomed.
Mater. Res. 66A, 93, 2003.
 Dohmen, P.M. et al., Tissue engineering of an auto-xenograft pulmonary heart valve, Asian
Cardiovasc. Thorac. Ann. 10, 25, 2002.
 Simon, P. et al., Early failure of the tissue engineered porcine heart valve SYNERGRAFT in pediatric
patients, Eur. J. Cardiothorac. Surg. 23, 1002, 2003.
 Steinhoff, G. et al., Tissue engineering of pulmonary heart valves on allogenic acellular matrix
conduits: in vivo restoration of valve tissue, Circulation 102, III50, 2000.
 Wilhelmi, M.H. et al., Role of inﬂammation and ischemia after implantation of xenogeneic
pulmonary valve conduits: histological evaluation after 6 to 12 months in sheep, Int. J. Artif.
Organs 26, 411, 2003.
 Leyh, R.G. et al., In vivo repopulation of xenogeneic and allogeneic acellular valve matrix conduits
in the pulmonary circulation, Ann. Thorac. Surg. 75, 1457, 2003.
 Curtil, A., Pegg, D.E., and Wilson, A., Repopulation of freeze-dried porcine valves with human
ﬁbroblasts and endothelial cells, J. Heart Valve Dis. 6, 296, 1997.
 O’Brien, M.F. et al., The SynerGraft valve: a new acellular (nonglutaraldehyde-ﬁxed) tissue heart
valve for autologous recellularization ﬁrst experimental studies before clinical implantation, Semin.
Thorac. Cardiovasc. Surg. 11, 194, 1999.
 Ye, Q. et al., Scaffold precoating with human autologous extracellular matrix for improved cell
attachment in cardiovascular tissue engineering, ASAIO J. 46, 730, 2000.
 Zund, G. et al., Tissue engineering in cardiovascular surgery: MTT, a rapid and reliable quantitative
method to assess the optimal human cell seeding on polymeric meshes, Eur. J. Cardiothorac. Surg.
15, 519, 1999.
 Shinoka, T. et al., Tissue-engineered heart valves. Autologous valve leaﬂet replacement study in a
lamb model, Circulation 94, II164, 1996.